The chapter presented several key concepts widely used throughout the thesis. The basics of nanowire growth have been introduced, with emphasis on the VLS mechanism. The chapter also presented some of the growth challenges of nanowire heterostructures via VLS technique. Lastly, III-V nanowire crystal phases were introduced including some of the reports on crystal phase control and the advantage of controlled polytypism.

34

**References**

[1] K. W. Adu, H. R. Gutiérrez, U. J. Kim, G. U. Sumanasekera, and P. C. Eklund, “Confined
phonons in Si nanowires.,” *Nano Lett.*, vol. 5, no. 3, pp. 409–14, 2005.

[2] A. R. Guichard, D. N. Barsic, S. Sharma, T. I. Kamins, and M. L. Brongersma, “Tunable
Light Emission from Quantum-Confined Excitons in TiSi 2 -Catalyzed Silicon
Nanowires,” *Nano Lett.*, vol. 6, no. 9, pp. 2140–2144, 2006.

[3] G. Koblmüller, K. Vizbaras, S. Hertenberger, S. Bolte, D. Rudolph, J. Becker, M.
Döblinger, M. C. Amann, J. J. Finley, and G. Abstreiter, “Diameter dependent optical
emission properties of InAs nanowires grown on Si,” *Appl. Phys. Lett.*, vol. 101, no. 5,
p. 053103, 2012.

[4] A. C. Ford, J. C. Ho, Y.-L. Chueh, Y.-C. Tseng, Z. Fan, J. Guo, J. Bokor, and A. Javey,
“Diameter-Dependent Electron Mobility of InAs Nanowires,” *Nano Lett.*, vol. 9, no. 1,
pp. 360–365, 2009.

[5] Y. Cui, Q. Wei, H. Park, and C. M. Lieber, “Nanowire nanosensors for highly sensitive
and selective detection of biological and chemical species.,” *Science*, vol. 293, no.
5533, pp. 1289–1292, 2001.

[6] P. Offermans, M. Crego-Calama, and S. H. Brongersma, “Gas detection with vertical
InAs nanowire arrays,” *Nano Lett.*, vol. 10, no. 7, pp. 2412–2415, 2010.

[7] M. W. Larsson, J. B. Wagner, M. Wallin, P. Håkansson, L. E. Fröberg, L. Samuelson, and L. R. Wallenberg, “Strain mapping in free-standing heterostructured wurtzite

InAs/InP nanowires,” *Nanotechnology*, vol. 18, no. 1, p. 015504, 2007.

[8] R. Chen, T.-T. D. Tran, K. W. Ng, W. S. Ko, L. C. Chuang, F. G. Sedgwick, and C. Chang-
Hasnain, “Nanolasers grown on silicon,” *Nat. Photonics*, vol. 5, pp. 170–175, 2011.
[9] F. Qian, Y. Li, S. Gradecak, H.-G. Park, Y. Dong, Y. Ding, Z. L. Wang, and C. M. Lieber,

“Multi-quantum-well nanowire heterostructures for wavelength-controlled lasers.,”

*Nat. Mater.*, vol. 7, no. 9, pp. 701–706, 2008.

[10] D. Saxena, S. Mokkapati, P. Parkinson, N. Jiang, Q. Gao, H. H. Tan, and C. Jagadish,
“Optically pumped room-temperature GaAs nanowire lasers,” *Nat. Photonics*, vol. 7,
no. 12, pp. 963–968, 2013.

[11] X. Duan, Y. Huang, R. Agarwal, and C. M. Lieber, “Single-nanowire electrically driven
lasers,” *Nature*, vol. 421, no. 6920, pp. 241–245, 2003.

[12] G. Larrieu and X.-L. Han, “Vertical nanowire array-based field effect transistors for
ultimate scaling,” *Nanoscale*, vol. 5, no. 6, pp. 2437–2441, 2013.

[13] L.-E. Wernersson, C. Thelander, E. Lind, and L. Samuelson, “III-V Nanowires -
Extending a Narrowing Road,” *Proc. IEEE*, vol. 98, no. 12, pp. 2047–2060, 2010.
[14] Y. Cui, Z. H. Zhong, D. L. Wang, W. U. Wang, and C. M. Lieber, “High performance

2. Basic concepts

35

[15] J. Xiang, W. Lu, Y. Hu, Y. Wu, H. Yan, and C. M. Lieber, “Ge/Si nanowire

heterostructures as high-performance field-effect transistors.,” *Nature*, vol. 441, no.
7092, pp. 489–493, 2006.

[16] C. Thelander, C. Rehnstedt, L. E. Froberg, E. Lind, T. Martensson, P. Caroff, T. Lowgren,
B. J. Ohlsson, L. Samuelson, and L.-E. Wernersson, “Development of a Vertical Wrap-
Gated InAs FET,” *IEEE Trans. Electron Devices*, vol. 55, no. 11, pp. 3030–3036, 2008.
[17] W. Lu, P. Xie, and C. M. Lieber, “Nanowire transistor performance limits and

applications,” *IEEE Trans. Electron Devices*, vol. 55, no. 11, pp. 2859–2876, 2008.
[18] K. Tomioka, M. Yoshimura, and T. Fukui, “A III–V nanowire channel on silicon for

high-performance vertical transistors,” *Nature*, vol. 488, no. 7410, pp. 189–192, 2012.
[19] A. L. Vallett, S. Minassian, P. Kaszuba, S. Datta, J. M. Redwing, and T. S. Mayer,

“Fabrication and Characterization of Axially Doped Silicon Nanowire Tunnel Field-
Effect Transistors,” *Nano Lett.*, vol. 10, no. 12, pp. 4813–4818, 2010.

[20] K. Tomioka, J. Motohisa, S. Hara, K. Hiruma, and T. Fukui, “GaAs/AlGaAs core

multishell nanowire-based light-emitting diodes on Si,” *Nano Lett.*, vol. 10, no. 5, pp.
1639–1644, 2010.

[21] C. P. T. Svensson, T. Mårtensson, J. Trägårdh, C. Larsson, M. Rask, D. Hessman, L.
Samuelson, and J. Ohlsson, “Monolithic GaAs/InGaP nanowire light emitting diodes
on silicon.,” *Nanotechnology*, vol. 19, no. 30, p. 305201, 2008.

[22] E. Dimakis, U. Jahn, M. Ramsteiner, A. Tahraoui, J. Grandal, X. Kong, O. Marquardt, A.
Trampert, H. Riechert, L. Geelhaar, M. Wu, X. Kong, M. Hanke, E. Dimakis, L. Geelhaar,
H. Riechert, J. Grandal, M. Wu, X. Kong, M. Hanke, and E. Dimakis, “Coaxial multishell
(In,Ga)As/GaAs nanowires for near-infrared emission on Si substrates,” *Nano Lett.*,
vol. 14, no. 5, pp. 2604–2609, 2014.

[23] J. V Holm, H. I. Jørgensen, P. Krogstrup, J. Nygård, H. Liu, and M. Aagesen, “Surface-
passivated GaAsP single-nanowire solar cells exceeding 10% efficiency grown on
silicon.,” *Nat. Commun.*, vol. 4, p. 1498, 2013.

[24] E. Nakai, M. Chen, M. Yoshimura, K. Tomioka, and T. Fukui, “InGaAs axial-junction
nanowire-array solar cells,” *Jpn. J. Appl. Phys.*, vol. 54, p. 015201, 2015.

[25] E. C. Garnett, M. L. Brongersma, Y. Cui, and M. D. McGehee, “Nanowire Solar Cells,”

*Annu. Rev. Mater. Res.*, vol. 41, no. 1, pp. 269–295, 2011.

[26] J. Svensson, N. Anttu, N. Vainorius, B. M. Borg, and L. E. Wernersson, “Diameter-
dependent photocurrent in InAsSb nanowire infrared photodetectors,” *Nano Lett.*,
vol. 13, no. 4, pp. 1380–1385, 2013.

[27] C. Soci, A. Zhang, X.-Y. Bao, H. Kim, Y. Lo, and D. Wang, “Nanowire photodetectors.,” *J. *
*Nanosci. Nanotechnol.*, vol. 10, no. 3, pp. 1430–1449, 2010.

[28] C. Cheng and H. J. Fan, “Branched nanowires: Synthesis and energy applications,”

36

[29] S. Xu, Y. Qin, C. Xu, Y. Wei, R. Yang, and Z. L. Wang, “Self-powered nanowire devices.,”

*Nat. Nanotechnol.*, vol. 5, no. 5, pp. 366–373, 2010.

[30] A. I. Hochbaum and P. Yang, “Semiconductor nanowires for energy conversion,”

*Nanoelectron. Conf. (INEC), 2010 3rd Int.*, pp. 527–546, 2010.

[31] A. I. Hochbaum, R. Chen, R. D. Delgado, W. Liang, E. C. Garnett, M. Najarian, A.
Majumdar, and P. Yang, “Enhanced thermoelectric performance of rough silicon
nanowires,” *Nature*, vol. 451, no. 7175, pp. 163–167, 2008.

[32] R. Yan, J.-H. Park, Y. Choi, C.-J. Heo, S.-M. Yang, L. P. Lee, and P. Yang, “Nanowire-based
single-cell endoscopy,” *Nat. Nanotechnol.*, vol. 7, no. 3, pp. 191–196, 2011.

[33] J. Arbiol, C. Magen, P. Becker, G. Jacopin, A. Chernikov, S. Schäfer, F. Furtmayr, M.
Tchernycheva, L. Rigutti, J. Teubert, S. Chatterjee, J. R. Morante, and M. Eickhoff, “Self-
assembled GaN quantum wires on GaN/AlN nanowire templates.,” *Nanoscale*, vol. 4,
no. 23, pp. 7517–24, 2012.

[34] M. Heiss, Y. Fontana, a Gustafsson, G. Wüst, C. Magen, D. D. O’Regan, J. W. Luo, B.
Ketterer, S. Conesa-Boj, a V Kuhlmann, J. Houel, E. Russo-Averchi, J. R. Morante, M.
Cantoni, N. Marzari, J. Arbiol, a Zunger, R. J. Warburton, and a Fontcuberta i Morral,
“Self-assembled quantum dots in a nanowire system for quantum photonics.,” *Nat. *
*Mater.*, vol. 12, no. 5, pp. 439–44, 2013.

[35] P. Caroff, M. E. Messing, B. Mattias Borg, K. A. Dick, K. Deppert, and L.-E. Wernersson, “InSb heterostructure nanowires: MOVPE growth under extreme lattice mismatch.,”

*Nanotechnology*, vol. 20, no. 49, p. 495606, 2009.

[36] M. Montazeri, M. Fickenscher, L. M. Smith, H. E. Jackson, J. Yarrison-rice, J. H. Kang, Q.
Gao, H. H. Tan, C. Jagadish, Y. Guo, J. Zou, M. Pistol, and C. E. Pryor, “Direct Measure of
Strain and Electronic Structure in GaAs / GaP Core - Shell Nanowires,” *Nano Lett.*, vol.
10, pp. 880–886, 2010.

[37] J. Treu, M. Bormann, H. Schmeiduch, M. Do, S. Morko, S. Matich, P. Wiecha, K. Saller, B.
Mayer, M. Bichler, M. Amann, J. J. Finley, G. Abstreiter, and G. Koblmu, “Enhanced
Luminescence Properties of InAs − InAsP Core − Shell Nanowires,” *Nano Lett.*, vol. 13,
no. 12, pp. 6070–6077, 2013.

[38] N. Skold, L. S. Karlsson, M. W. Larsson, M. Pistol, W. Seifert, and J. Tra, “Growth and
Optical Properties of Strained GaAs − GaxIn1 - xP Core − Shell Nanowires,” *Nano Lett.*,
vol. 5, no. 10, pp. 1943–1947, 2005.

[39] M. E. Pistol and C. E. Pryor, “Band structure of core-shell semiconductor nanowires,”

*Phys. Rev. B - Condens. Matter Mater. Phys.*, vol. 78, no. 11, pp. 1–12, 2008.

[40] R. S. Wagner and W. C. Ellis, “Vapor-liquid-solid mechanism of single crystal growth,”

*Appl. Phys. Lett.*, vol. 4, no. 5, pp. 89–90, 1964.

[41] X. Duan and C. M. Lieber, “General synthesis of compound semiconductor nanowires,”

2. Basic concepts

37

[42] C.-C. Chen, C.-C. Yeh, C.-H. Chen, M.-Y. Yu, H.-L. Liu, J.-J. Wu, K.-H. Chen, L.-C. Chen, J.-Y.
Peng, and Y.-F. Chen, “Catalytic Growth and Characterization of Gallium Nitride
Nanowires,” *J. Am. Chem. Soc.*, vol. 123, no. 12, pp. 2791–2798, 2001.

[43] J. Arbiol, B. Kalache, P. R. i Cabarrocas, J. R. Morante, and A. F. i Morral, “Influence of
Cu as a catalyst on the properties of silicon nanowires synthesized by the vapour–
solid–solid mechanism,” *Nanotechnology*, vol. 18, no. 30, p. 305606, 2007.

[44] X. Weng, R. a Burke, and J. M. Redwing, “The nature of catalyst particles and growth
mechanisms of GaN nanowires grown by Ni-assisted metal–organic chemical vapor
deposition,” *Nanotechnology*, vol. 20, no. 8, p. 085610, 2009.

[45] C. Colombo, D. Spirkoska, M. Frimmer, G. Abstreiter, and a. Fontcuberta I Morral, “Ga-
assisted catalyst-free growth mechanism of GaAs nanowires by molecular beam
epitaxy,” *Phys. Rev. B - Condens. Matter Mater. Phys.*, vol. 77, no. 15, pp. 2–6, 2008.
[46] K. Tomioka, K. Ikejiri, T. Tanaka, J. Motohisa, S. Hara, K. Hiruma, and T. Fukui,

“Selective-area growth of III-V nanowires and their applications,” *J. Mater. Res.*, vol.
26, no. 17, pp. 2127–2141, 2011.

[47] J. Bolinsson, P. Caroff, B. Mandl, and K. A. Dick, “Wurtzite-zincblende superlattices in
InAs nanowires using a supply interruption method.,” *Nanotechnology*, vol. 22, no. 26,
p. 265606, 2011.

[48] K. A. Dick, P. Caroff, J. Bolinsson, M. E. Messing, J. Johansson, K. Deppert, L. R.

Wallenberg, and L. Samuelson, “Control of III–V nanowire crystal structure by growth
parameter tuning,” *Semicond. Sci. Technol.*, vol. 25, no. 2, p. 024009, 2010.

[49] P. Caroff, J. Bolinsson, and J. Johansson, “Crystal phases in III-V nanowires: From
random toward engineered polytypism,” *IEEE J. Sel. Top. Quantum Electron.*, vol. 17,
no. 4, pp. 829–846, 2011.

[50] H. J. Joyce, Q. Gao, J. Wong-Leung, Y. Kim, H. H. Tan, and C. Jagadish, “Tailoring GaAs,
InAs, and InGaAs nanowires for optoelectronic device applications,” *IEEE J. Sel. Top. *
*Quantum Electron.*, vol. 17, no. 4, pp. 766–778, 2011.

[51] S. Hofmann, R. Sharma, C. T. Wirth, F. Cervantes-Sodi, C. Ducati, T. Kasama, R. E.
Dunin-Borkowski, J. Drucker, P. Bennett, and J. Robertson, “Ledge-flow-controlled
catalyst interface dynamics during Si nanowire growth,” *Nat. Mater.*, vol. 7, no. 5, pp.
372–375, 2008.

[52] B. A. Wacaser, K. A. Dick, J. Johansson, M. T. Borgström, K. Deppert, and L. Samuelson,
“Preferential interface nucleation: An expansion of the VLS growth mechanism for
nanowires,” *Adv. Mater.*, vol. 21, no. 2, pp. 153–165, 2009.

[53] F. Glas, “Chemical potentials for Au-assisted vapor-liquid-solid growth of III-V
nanowires,” *J. Appl. Phys.*, vol. 108, no. 7, p. 073506, 2010.

[54] V. a. Nebol’sin and a. a. Shchetinin, “Role of Surface Energy in the Vapor – Liquid –
Solid Growth of Silicon,” *Inorg. Mater.*, vol. 39, no. 9, pp. 899–903, 2003.

38

[55] B. A. Wacaser, K. Deppert, L. S. Karlsson, L. Samuelson, and W. Seifert, “Growth and
characterization of defect free GaAs nanowires,” *J. Cryst. Growth*, vol. 287, no. 2, pp.
504–508, 2006.

[56] C.-Y. Wen, J. Tersoff, M. C. Reuter, E. A. Stach, and F. M. Ross, “Step-Flow Kinetics in
Nanowire Growth,” *Phys. Rev. Lett.*, vol. 105, no. 19, p. 195502, 2010.

[57] K. Kolasinski, “Catalytic growth of nanowires: Vapor–liquid–solid, vapor–solid–solid,
solution–liquid–solid and solid–liquid–solid growth,” *Curr. Opin. Solid State Mater. *
*Sci.*, vol. 10, no. 3–4, pp. 182–191, 2006.

[58] T. C. Thomas and R. S. Williams, “Solid phase equilibria in the Au-Ga-As, Au-Ga-Sb, Au-
In-As, and Au-In-Sb ternaries,” *J. Mater. Res.*, vol. 1, no. 02, pp. 352–360, 1986.

[59] C. Chatillon, F. Hodaj, and a. Pisch, “Thermodynamics of GaAs nanowire MBE growth
with gold droplets,” *J. Cryst. Growth*, vol. 311, no. 14, pp. 3598–3608, 2009.

[60] M. Tchernycheva, J. C. Harmand, G. Patriarche, L. Travers, and G. E. Cirlin,

“Temperature conditions for GaAs nanowire formation by Au-assisted molecular
beam epitaxy.,” *Nanotechnology*, vol. 17, no. 16, pp. 4025–4030, 2006.

[61] M. Ghasemi, B. Sundman, S. G. Fries, and J. Johansson, “The thermodynamic
assessment of the Au-In-Ga system,” *J. Alloys Compd.*, vol. 600, pp. 178–185, 2014.
[62] S. G. Ghalamestani, M. Ek, M. Ghasemi, P. Caroff, J. Johansson, and K. a. Dick,

“Morphology and composition controlled Ga x In 1−x Sb nanowires: understanding
ternary antimonide growth,” *Nanoscale*, vol. 6, no. 2, pp. 1086–1092, 2014.

[63] K. A. Dick, K. Deppert, L. S. Karlsson, L. R. Wallenberg, L. Samuelson, and W. Seifert, “A
New Understanding of Au-Assisted Growth of III-V Semiconductor Nanowires,” *Adv. *
*Funct. Mater.*, vol. 15, no. 10, pp. 1603–1610, 2005.

[64] P. J. Poole, D. Dalacu, X. Wu, J. Lapointe, and K. Mnaymneh, “Interplay between crystal
phase purity and radial growth in InP nanowires,” *Nanotechnology*, vol. 23, no. 38, p.
385205, 2012.

[65] S. Gorji Ghalamestani, M. Heurlin, L.-E. Wernersson, S. Lehmann, and K. A. Dick, “Growth of InAs/InP core-shell nanowires with various pure crystal structures.,”

*Nanotechnology*, vol. 23, no. 28, p. 285601, 2012.

[66] M. A. Verheijen, G. Immink, T. De Smet, M. T. Borgström, and E. P. a M. Bakkers,
“Growth kinetics of heterostructured GaP-GaAs nanowires,” *J. Am. Chem. Soc.*, vol.
128, no. 9, pp. 1353–1359, 2006.

[67] J. Johansson, C. P. T. Svensson, T. Mårtensson, L. Samuelson, and W. Seifert, “Mass
transport model for semiconductor nanowire growth.,” *J. Phys. Chem. B*, vol. 109, no.
28, pp. 13567–13571, 2005.

[68] V. G. Dubrovskii, N. V. Sibirev, R. a. Suris, G. E. Cirlin, J. C. Harmand, and V. M. Ustinov,
“Diffusion-controlled growth of semiconductor nanowires: Vapor pressure versus
high vacuum deposition,” *Surf. Sci.*, vol. 601, no. 18, pp. 4395–4401, 2007.

2. Basic concepts

39

[69] L. E. Jensen, M. T. Bjo, A. I. Persson, B. J. Ohlsson, and L. Samuelson, “Role of Surface
Diffusion in Chemical Beam Epitaxy of InAs Nanowires,” *Nano Lett.*, vol. 4, no. 10, pp.
1961–1964, 2004.

[70] M. Paladugu, J. Zou, Y. N. Guo, X. Zhang, Y. Kim, H. J. Joyce, Q. Gao, H. H. Tan, and C.
Jagadish, “Nature of heterointerfaces in GaAs/InAs and InAs/GaAs axial nanowire
heterostructures,” *Appl. Phys. Lett.*, vol. 93, no. 10, p. 101911, 2008.

[71] D. E. Perea, N. Li, R. M. Dickerson, A. Misra, and S. T. Picraux, “Controlling
heterojunction abruptness in VLS-grown semiconductor nanowires via in situ
catalyst alloying,” *Nano Lett.*, vol. 11, no. 8, pp. 3117–3122, 2011.

[72] K. A. Dick, J. Bolinsson, B. M. Borg, and J. Johansson, “Controlling the Abruptness of
Axial Heterojunctions in III−V Nanowires: Beyond the Reservoir Effect,” *Nano Lett.*,
vol. 12, no. 6, pp. 3200–3206, 2012.

[73] N. Jiang, Q. Gao, P. Parkinson, J. Wong-Leung, S. Mokkapati, S. Breuer, H. H. Tan, C. L. Zheng, J. Etheridge, and C. Jagadish, “Enhanced minority carrier lifetimes in

GaAs/AlGaAs core-shell nanowires through shell growth optimization,” *Nano Lett.*,
vol. 13, no. 11, pp. 5135–5140, 2013.

[74] M. Paladugu, J. Zou, Y. N. Guo, G. J. Auchterlonie, H. J. Joyce, Q. Gao, H. H. Tan, C.
Jagadish, and Y. Kim, “Novel growth phenomena observed in axial InAs/GaAs
nanowire heterostructures,” *Small*, vol. 3, no. 11, pp. 1873–1877, 2007.

[75] M. E. Messing, J. Wong-Leung, Z. Zanolli, H. J. Joyce, H. H. Tan, Q. Gao, L. R. Wallenberg, J. Johansson, and C. Jagadish, “Growth of straight InAs-on-GaAs nanowire

heterostructures,” *Nano Lett.*, vol. 11, no. 9, pp. 3899–3905, 2011.

[76] K. A. Dick, S. Kodambaka, M. C. Reuter, K. Deppert, L. Samuelson, W. Seifert, L. R.
Wallenberg, and F. M. Ross, “The morphology of axial and branched nanowire
heterostructures,” *Nano Lett.*, vol. 7, no. 6, pp. 1817–1822, 2007.

[77] R. E. Algra, M. Hocevar, M. A. Verheijen, I. Zardo, G. G. W. Immink, W. J. P. van

Enckevort, G. Abstreiter, L. P. Kouwenhoven, E. Vlieg, and E. P. A. M. Bakkers, “Crystal
structure transfer in core/shell nanowires.,” *Nano Lett.*, vol. 11, no. 4, pp. 1690–4,
2011.

[78] S. G. Ghalamestani, a M. Munshi, D. L. Dheeraj, B.-O. Fimland, H. Weman, and K. A.
Dick, “Self-catalyzed MBE grown GaAs/GaAsxSb1-x core-shell nanowires in ZB and
WZ crystal structures.,” *Nanotechnology*, vol. 24, no. 40, p. 405601, 2013.

[79] T. Rieger, T. Schäpers, D. Grützmacher, and M. I. Lepsa, “Crystal Phase Selective
Growth in GaAs/InAs Core–Shell Nanowires,” *Cryst. Growth Des.*, vol. 14, no. 3, pp.
1167–1174, 2014.

[80] K. L. Kavanagh, I. Saveliev, M. Blumin, G. Swadener, and H. E. Ruda, “Faster radial
strain relaxation in InAs-GaAs core-shell heterowires,” *J. Appl. Phys.*, vol. 111, no. 4, p.
044301, 2012.

40

[81] H. Chu, C. Zhou, J. Wang, and I. J. Beyerlein, “Misfit strain relaxation mechanisms in
core/shell nanowires,” *JOM J. Miner. Met. Mater. Soc.*, vol. 64, no. 10, pp. 1258–1262,
2012.

[82] K. E. Aifantis, a. L. Kolesnikova, and a. E. Romanov, “Nucleation of misfit dislocations
and plastic deformation in core/shell nanowires,” *Philos. Mag.*, vol. 87, no. 30, pp.
4731–4757, 2007.

[83] I. A. Goldthorpe, A. F. Marshall, and P. C. McIntyre, “Synthesis and strain relaxation of
Ge-core/Si-shell nanowire arrays,” *Nano Lett.*, vol. 8, no. 11, pp. 4081–4086, 2008.
[84] S. Conesa-Boj, H. I. T. Hauge, M. A. Verheijen, S. Assali, A. Li, E. P. A. M. Bakkers, and A.

Fontcuberta i Morral, “Cracking the Si Shell Growth in Hexagonal GaP-Si Core–Shell
Nanowires,” *Nano Lett.*, vol. 15, no. 5, pp. 2974–2979, 2015.

[85] M. J. L. Sourribes, I. Isakov, M. Pan, H. Liu, and P. A. Warburton, “Mobility
Enhancement by Sb-mediated Minimisation of Stacking Fault Density in InAs
Nanowires Grown on Silicon Growth of InAs and InAsSb nanowires,” *Nano Lett.*, vol.
14, no. 1, pp. 1–10, 2014.

[86] S. Morkötter, S. Funk, M. Liang, M. Döblinger, S. Hertenberger, J. Treu, D. Rudolph, A.
Yadav, J. Becker, M. Bichler, G. Scarpa, P. Lugli, I. Zardo, J. J. Finley, G. Abstreiter, and G.
Koblmüller, “Role of microstructure on optical properties in high-uniformity In1-
xGaxAs nanowire arrays: Evidence of a wider wurtzite band gap,” *Phys. Rev. B - *

*Condens. Matter Mater. Phys.*, vol. 87, no. 20, pp. 1–9, 2013.

[87] C. Thelander, P. Caroff, S. Plissard, A. W. Dey, and K. A. Dick, “Effects of crystal phase
mixing on the electrical properties of InAs nanowires,” *Nano Lett.*, vol. 11, no. 6, pp.
2424–2429, 2011.

[88] D. Spirkoska, J. Arbiol, A. Gustafsson, S. Conesa-Boj, F. Glas, I. Zardo, M. Heigoldt, M. H. Gass, A. L. Bleloch, S. Estrade, M. Kaniber, J. Rossler, F. Peiro, J. R. Morante, G.

Abstreiter, L. Samuelson, and A. Fontcuberta I Morral, “Structural and optical properties of high quality zinc-blende/wurtzite GaAs nanowire heterostructures,”

*Phys. Rev. B - Condens. Matter Mater. Phys.*, vol. 80, no. 24, pp. 1–9, 2009.

[89] J.-M. M. Jancu, K. Gauthron, L. Largeau, G. Patriarche, J.-C. C. Harmand, and P. Voisin,
“Type II heterostructures formed by zinc-blende inclusions in InP and GaAs wurtzite
nanowires,” *Appl. Phys. Lett.*, vol. 97, no. 4, p. 041910, 2010.

[90] K. Pemasiri, M. Montazeri, R. Gass, L. M. Smith, H. E. Jackson, J. Yarrison-Rice, S.
Paiman, Q. Gao, H. H. Tan, C. Jagadish, X. Zhang, and J. Zou, “Carrier dynamics and
quantum confinement in type II ZB-WZ InP nanowire homostructures,” *Nano Lett.*,
vol. 9, no. 2, pp. 648–654, 2009.

[91] L. Zhang, J. W. Luo, A. Zunger, N. Akopian, V. Zwiller, and J. C. Harmand, “Wide InP Nanowires with wurtzite/zincblende superlattice segments are type-II whereas